# Electronic Supplementary Material (ESI) for CrystEngComm.
# This journal is © The Royal Society of Chemistry 2022

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_RbAgF3
_database_code_depnum_ccdc_archive 'CCDC 2122449'
loop_
_audit_author_name
_audit_author_address
'Kacper Koteras'
;Centre of New Technologies University of Warsaw
Poland
;
_audit_update_record             
;
2021-11-18 deposited with the CCDC.	2021-12-23 downloaded from the CCDC.
;
# start Validation Reply Form
_vrf_PLAT113_RbAgF3              
;
PROBLEM: ADDSYM Suggests Possible Pseudo/New  Space Group     P4/mmm Check
RESPONSE: The primitive cell suggested by this alert is certainly wrong as it  has equal equatorial Ag-F bonds within AgF2 sheets; this does not happen in any  compound of Ag(II) since - due to cooperative Jahn-Teller effect - the Ag-F bond  pattern is antiferrodistortive, i.e. long-short-long-short etc. The only  exception from that would be a system with strong substitutional disorder  reflected by two distinct positions of F atoms inside the plane, both occupied with 50% probability. this model is hard to be differentiated from our model  solely in a Rietveld fit. as we see no support for such a disordered model from  other methods we decided to use ordered I-centered cell.
;
_vrf_REFI015_RbAgF3              
;
PROBLEM: _refine_ls_shift/su_max is missing
RESPONSE: FullProf software doesn't provide that particular parameter, as it  reports them equal to zero after reaching convergence.
;
_vrf_PLAT741_RbAgF3              
;
PROBLEM: Bond    Calc 3.16930(10), Rep     3.16928 ......    Missing s.u.
RESPONSE: This are the distances between atoms in special positions, so  FullProf doesn't add standard uncertainties to them.
;
_vrf_PLAT752_RbAgF3              
;
PROBLEM: Angle   Calc       90.00, Rep    90.0(10) ......  Senseless s.u.
RESPONSE: This is an error caused by Fullprof numerical methods.
;
# Added during the CSD deposition process: Thursday 18 November 2021 01:57 PM
# end Validation Reply Form


#=============================================================================

# 5. CHEMICAL DATA

_chemical_name_systematic        'Rubidium trifluoroargentate(II)'
_chemical_formula_structural     'Ag F3 Rb'
_chemical_formula_iupac          'Ag F3 Rb'
_chemical_formula_sum            'Ag F3 Rb'
_chemical_formula_weight         250.3310
_exptl_crystal_density_diffrn    4.905


#=============================================================================

# 6. POWDER SPECIMEN AND CRYSTAL DATA

_symmetry_cell_setting           Tetragonal
_symmetry_space_group_name_H-M   'I 4/m c m'
_symmetry_space_group_name_Hall  '-I 4 2c'

loop_
_symmetry_equiv_pos_as_xyz #<--must include 'x,y,z'
x,y,z
-y,x,z
-x,-y,z
y,-x,z
-x,y,z+1/2
y,x,z+1/2
x,-y,z+1/2
-y,-x,z+1/2
-x,-y,-z
y,-x,-z
x,y,-z
-y,x,-z
x,-y,-z+1/2
-y,-x,-z+1/2
-x,y,-z+1/2
y,x,-z+1/2
x+1/2,y+1/2,z+1/2
-y+1/2,x+1/2,z+1/2
-x+1/2,-y+1/2,z+1/2
y+1/2,-x+1/2,z+1/2
-x+1/2,y+1/2,z
y+1/2,x+1/2,z
x+1/2,-y+1/2,z
-y+1/2,-x+1/2,z
-x+1/2,-y+1/2,-z+1/2
y+1/2,-x+1/2,-z+1/2
x+1/2,y+1/2,-z+1/2
-y+1/2,x+1/2,-z+1/2
x+1/2,-y+1/2,-z
-y+1/2,-x+1/2,-z
-x+1/2,y+1/2,-z
y+1/2,x+1/2,-z

_cell_length_a                   6.33855(6)
_cell_length_b                   6.33855(6)
_cell_length_c                   8.43740(11)
_cell_angle_alpha                90.0000
_cell_angle_beta                 90.0000
_cell_angle_gamma                90.0000
_cell_volume                     338.991(6)
_cell_formula_units_Z            4
_cell_measurement_temperature    293
_cell_special_details            
; ?
;


# The next five fields are character fields that describe the specimen.

_pd_spec_mounting                capillary # This field should be
# used to give details of the 
# container.
_pd_spec_mount_mode              transmission # options are 'reflection'
# or 'transmission'
_pd_spec_shape                   cylinder # options are 'cylinder' 
# 'flat_sheet' or 'irregular'
_pd_char_colour                  brown # use ICDD colour descriptions


#=============================================================================

# 7. EXPERIMENTAL DATA


# The following item is used to identify the equipment used to record 
# the powder pattern when the diffractogram was measured at a laboratory 
# other than the authors' home institution, e.g. when neutron or synchrotron
# radiation is used.

_diffrn_ambient_temperature      293
_diffrn_radiation_type           'Cu K\a'

_diffrn_radiation_monochromator  none
_diffrn_measurement_device_type  'Bruker D8 DISCOVER'
_diffrn_measurement_method       capillary
_pd_meas_scan_method             step # options are 'step', 'cont',
# 'tof', 'fixed' or
# 'disp' (= dispersive)
_pd_meas_special_details         ?

#  The following four items give details of the measured (not processed)
#  powder pattern.  Angles are in degrees.

_pd_meas_number_of_points        5866
_pd_meas_2theta_range_min        6.01430
_pd_meas_2theta_range_max        89.86021
_pd_meas_2theta_range_inc        0.014299

#=============================================================================

# 8. REFINEMENT DATA

_refine_special_details          ?

# Use the next field to give any special details about the fitting of the
# powder pattern.

_pd_proc_ls_special_details      ?

# The next three items are given as text.

_pd_proc_ls_profile_function     ?
_pd_proc_ls_background_function  ?
_pd_proc_ls_pref_orient_corr     ?

#  The following profile R-factors are NOT CORRECTED for background
#  The sum is extended to all non-excluded points.
#  These are the current CIF standard

_pd_proc_ls_prof_R_factor        0.8424
_pd_proc_ls_prof_wR_factor       1.7781
_pd_proc_ls_prof_wR_expected     0.5940


#  Items related to LS refinement

_refine_ls_goodness_of_fit_all   2.99
_refine_ls_R_I_factor            9.5332
_refine_ls_number_reflns         95
_refine_ls_number_parameters     18
_refine_ls_number_restraints     0

# The following four items apply to angular dispersive measurements.
# 2theta minimum, maximum and increment (in degrees) are for the 
# intensities used in the refinement.

_pd_proc_2theta_range_min        6.0151
_pd_proc_2theta_range_max        89.8610
_pd_proc_2theta_range_inc        0.014299
_pd_proc_wavelength              1.540560


loop_
_pd_block_diffractogram_id
?
# The id used for the block containing
# the powder pattern profile (section 11)

# Give appropriate details in the next two text fields.

_pd_proc_info_excluded_regions   none
_pd_proc_info_data_reduction     none

# The following items are used to identify the programs used.

_computing_data_collection       ?
_computing_structure_solution    ?
_computing_structure_refinement  FULLPROF
_computing_molecular_graphics    ?
_computing_publication_material  ?

#=============================================================================

# 9. ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS

loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_occupancy
_atom_site_adp_type
_atom_site_type_symbol

Rb1 0.00000 0.00000 0.25000 0.0100(11) 1.00000 Uiso Rb
Ag1 0.00000 0.50000 0.00000 0.0043(8) 1.00000 Uiso Ag
F1 0.00000 0.50000 0.25000 0.010(3) 1.00000 Uiso F
F2 0.240(4) 0.740(4) 0.00000 0.017(3) 1.00000 Uiso F


# Note: if the displacement parameters were refined anisotropically
# the U matrices should be given as for single-crystal studies.

#=============================================================================

# 10. DISTANCES AND ANGLES / MOLECULAR GEOMETRY 
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Rb1 F1 3.16928 1_545 ?
Rb1 F1 3.16928 1_555 ?
Rb1 F1 3.16928 2_555 ?
Rb1 F1 3.16928 2_655 ?
Rb1 F2 3.079(18) 1_545 ?
Rb1 F2 3.079(18) 2_655 ?
Rb1 F2 3.079(18) 3_565 ?
Rb1 F2 3.079(18) 4_455 ?
Rb1 F2 3.079(18) 5_545 ?
Rb1 F2 3.079(18) 6_455 ?
Rb1 F2 3.079(18) 7_565 ?
Rb1 F2 3.079(18) 8_655 ?
Ag1 F1 2.10935 1_555 ?
Ag1 F1 2.10935 5_554 ?
Ag1 F2 2.15(3) 1_555 ?
Ag1 F2 2.33(3) 2_655 ?
Ag1 F2 2.15(3) 3_565 ?
Ag1 F2 2.33(3) 4_465 ?
F1 Rb1 3.16928 1_555 ?
F1 Rb1 3.16928 1_565 ?
F1 Rb1 3.16928 21_455 ?
F1 Rb1 3.16928 21_555 ?
F1 Ag1 2.10935 1_555 ?
F1 Ag1 2.10935 5_555 ?
F1 F2 3.013(18) 1_555 ?
F1 F2 3.143(19) 2_655 ?
F1 F2 3.013(18) 3_565 ?
F1 F2 3.143(19) 4_465 ?
F1 F2 3.013(18) 5_555 ?
F1 F2 3.143(19) 6_455 ?
F1 F2 3.013(18) 7_565 ?
F1 F2 3.143(19) 8_665 ?
F2 Rb1 3.079(18) 1_565 ?
F2 Rb1 3.079(18) 5_564 ?
F2 Rb1 3.079(18) 17_554 ?
F2 Rb1 3.079(18) 21_555 ?
F2 Ag1 2.15(3) 1_555 ?
F2 Ag1 2.33(3) 2_665 ?
F2 F1 3.013(18) 1_555 ?
F2 F1 3.143(19) 2_665 ?
F2 F1 3.013(18) 5_554 ?
F2 F1 3.143(19) 6_564 ?
F2 F2 3.17(4) 2_655 ?
F2 F2 3.17(4) 2_665 ?
F2 F2 3.17(4) 4_465 ?
F2 F2 3.17(4) 4_565 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
F1 Rb1 F1 180.000 1_545 1_555 ?
F1 Rb1 F1 90.0000 1_545 2_555 ?
F1 Rb1 F1 90.0000 1_545 2_655 ?
F1 Rb1 F2 57.6(5) 1_545 1_545 ?
F1 Rb1 F2 119.6(8) 1_545 2_655 ?
F1 Rb1 F2 122.4(8) 1_545 3_565 ?
F1 Rb1 F2 60.4(5) 1_545 4_455 ?
F1 Rb1 F2 57.6(5) 1_545 5_545 ?
F1 Rb1 F2 119.6(8) 1_545 6_455 ?
F1 Rb1 F2 122.4(8) 1_545 7_565 ?
F1 Rb1 F2 60.4(5) 1_545 8_655 ?
F1 Rb1 F1 90.0000 1_555 2_555 ?
F1 Rb1 F1 90.0000 1_555 2_655 ?
F1 Rb1 F2 122.4(8) 1_555 1_545 ?
F1 Rb1 F2 60.4(5) 1_555 2_655 ?
F1 Rb1 F2 57.6(5) 1_555 3_565 ?
F1 Rb1 F2 119.6(8) 1_555 4_455 ?
F1 Rb1 F2 122.4(8) 1_555 5_545 ?
F1 Rb1 F2 60.4(5) 1_555 6_455 ?
F1 Rb1 F2 57.6(5) 1_555 7_565 ?
F1 Rb1 F2 119.6(8) 1_555 8_655 ?
F1 Rb1 F1 180.000 2_555 2_655 ?
F1 Rb1 F2 119.6(8) 2_555 1_545 ?
F1 Rb1 F2 122.4(8) 2_555 2_655 ?
F1 Rb1 F2 60.4(5) 2_555 3_565 ?
F1 Rb1 F2 57.6(5) 2_555 4_455 ?
F1 Rb1 F2 60.4(5) 2_555 5_545 ?
F1 Rb1 F2 57.6(5) 2_555 6_455 ?
F1 Rb1 F2 119.6(8) 2_555 7_565 ?
F1 Rb1 F2 122.4(8) 2_555 8_655 ?
F1 Rb1 F2 60.4(5) 2_655 1_545 ?
F1 Rb1 F2 57.6(5) 2_655 2_655 ?
F1 Rb1 F2 119.6(8) 2_655 3_565 ?
F1 Rb1 F2 122.4(8) 2_655 4_455 ?
F1 Rb1 F2 119.6(8) 2_655 5_545 ?
F1 Rb1 F2 122.4(8) 2_655 6_455 ?
F1 Rb1 F2 60.4(5) 2_655 7_565 ?
F1 Rb1 F2 57.6(5) 2_655 8_655 ?
F2 Rb1 F2 62.0(8) 1_545 2_655 ?
F2 Rb1 F2 93.5(11) 1_545 3_565 ?
F2 Rb1 F2 62.0(8) 1_545 4_455 ?
F2 Rb1 F2 115.3(8) 1_545 5_545 ?
F2 Rb1 F2 176.7(11) 1_545 6_455 ?
F2 Rb1 F2 120.8(9) 1_545 7_565 ?
F2 Rb1 F2 86.6(5) 1_545 8_655 ?
F2 Rb1 F2 62.0(8) 2_655 3_565 ?
F2 Rb1 F2 93.5(11) 2_655 4_455 ?
F2 Rb1 F2 176.7(11) 2_655 5_545 ?
F2 Rb1 F2 120.8(9) 2_655 6_455 ?
F2 Rb1 F2 86.6(5) 2_655 7_565 ?
F2 Rb1 F2 115.3(8) 2_655 8_655 ?
F2 Rb1 F2 62.0(8) 3_565 4_455 ?
F2 Rb1 F2 120.8(9) 3_565 5_545 ?
F2 Rb1 F2 86.6(5) 3_565 6_455 ?
F2 Rb1 F2 115.3(8) 3_565 7_565 ?
F2 Rb1 F2 176.7(11) 3_565 8_655 ?
F2 Rb1 F2 86.6(5) 4_455 5_545 ?
F2 Rb1 F2 115.3(8) 4_455 6_455 ?
F2 Rb1 F2 176.7(11) 4_455 7_565 ?
F2 Rb1 F2 120.8(9) 4_455 8_655 ?
F2 Rb1 F2 62.0(8) 5_545 6_455 ?
F2 Rb1 F2 93.5(11) 5_545 7_565 ?
F2 Rb1 F2 62.0(8) 5_545 8_655 ?
F2 Rb1 F2 62.0(8) 6_455 7_565 ?
F2 Rb1 F2 93.5(11) 6_455 8_655 ?
F2 Rb1 F2 62.0(8) 7_565 8_655 ?
F1 Ag1 F1 180.000 1_555 5_554 ?
F1 Ag1 F2 90.0(10) 1_555 1_555 ?
F1 Ag1 F2 90.0(9) 1_555 2_655 ?
F1 Ag1 F2 90.0(10) 1_555 3_565 ?
F1 Ag1 F2 90.0(9) 1_555 4_465 ?
F1 Ag1 F2 90.0(10) 5_554 1_555 ?
F1 Ag1 F2 90.0(9) 5_554 2_655 ?
F1 Ag1 F2 90.0(10) 5_554 3_565 ?
F1 Ag1 F2 90.0(9) 5_554 4_465 ?
F2 Ag1 F2 90.0(16) 1_555 2_655 ?
F2 Ag1 F2 180(2) 1_555 3_565 ?
F2 Ag1 F2 90.0(16) 1_555 4_465 ?
F2 Ag1 F2 90.0(16) 2_655 3_565 ?
F2 Ag1 F2 180.0(20) 2_655 4_465 ?
F2 Ag1 F2 90.0(16) 3_565 4_465 ?
Rb1 F1 Rb1 180.000 1_555 1_565 ?
Rb1 F1 Rb1 90.0000 1_555 21_455 ?
Rb1 F1 Rb1 90.0000 1_555 21_555 ?
Rb1 F1 Ag1 90.0000 1_555 1_555 ?
Rb1 F1 Ag1 90.0000 1_555 5_555 ?
Rb1 F1 F2 120.3(8) 1_555 1_555 ?
Rb1 F1 F2 58.4(5) 1_555 2_655 ?
Rb1 F1 F2 59.7(5) 1_555 3_565 ?
Rb1 F1 F2 121.6(8) 1_555 4_465 ?
Rb1 F1 F2 120.3(8) 1_555 5_555 ?
Rb1 F1 F2 58.4(5) 1_555 6_455 ?
Rb1 F1 F2 59.7(5) 1_555 7_565 ?
Rb1 F1 F2 121.6(8) 1_555 8_665 ?
Rb1 F1 Rb1 90.0000 1_565 21_455 ?
Rb1 F1 Rb1 90.0000 1_565 21_555 ?
Rb1 F1 Ag1 90.0000 1_565 1_555 ?
Rb1 F1 Ag1 90.0000 1_565 5_555 ?
Rb1 F1 F2 59.7(5) 1_565 1_555 ?
Rb1 F1 F2 121.6(8) 1_565 2_655 ?
Rb1 F1 F2 120.3(8) 1_565 3_565 ?
Rb1 F1 F2 58.4(5) 1_565 4_465 ?
Rb1 F1 F2 59.7(5) 1_565 5_555 ?
Rb1 F1 F2 121.6(8) 1_565 6_455 ?
Rb1 F1 F2 120.3(8) 1_565 7_565 ?
Rb1 F1 F2 58.4(5) 1_565 8_665 ?
Rb1 F1 Rb1 180.000 21_455 21_555 ?
Rb1 F1 Ag1 90.0000 21_455 1_555 ?
Rb1 F1 Ag1 90.0000 21_455 5_555 ?
Rb1 F1 F2 120.3(8) 21_455 1_555 ?
Rb1 F1 F2 121.6(8) 21_455 2_655 ?
Rb1 F1 F2 59.7(5) 21_455 3_565 ?
Rb1 F1 F2 58.4(5) 21_455 4_465 ?
Rb1 F1 F2 59.7(5) 21_455 5_555 ?
Rb1 F1 F2 58.4(5) 21_455 6_455 ?
Rb1 F1 F2 120.3(8) 21_455 7_565 ?
Rb1 F1 F2 121.6(8) 21_455 8_665 ?
Rb1 F1 Ag1 90.0000 21_555 1_555 ?
Rb1 F1 Ag1 90.0000 21_555 5_555 ?
Rb1 F1 F2 59.7(5) 21_555 1_555 ?
Rb1 F1 F2 58.4(5) 21_555 2_655 ?
Rb1 F1 F2 120.3(8) 21_555 3_565 ?
Rb1 F1 F2 121.6(8) 21_555 4_465 ?
Rb1 F1 F2 120.3(8) 21_555 5_555 ?
Rb1 F1 F2 121.6(8) 21_555 6_455 ?
Rb1 F1 F2 59.7(5) 21_555 7_565 ?
Rb1 F1 F2 58.4(5) 21_555 8_665 ?
Ag1 F1 Ag1 180.000 1_555 5_555 ?
Ag1 F1 F2 45.6(6) 1_555 1_555 ?
Ag1 F1 F2 47.9(6) 1_555 2_655 ?
Ag1 F1 F2 45.6(6) 1_555 3_565 ?
Ag1 F1 F2 47.9(6) 1_555 4_465 ?
Ag1 F1 F2 134.4(6) 1_555 5_555 ?
Ag1 F1 F2 132.1(6) 1_555 6_455 ?
Ag1 F1 F2 134.4(6) 1_555 7_565 ?
Ag1 F1 F2 132.1(6) 1_555 8_665 ?
Ag1 F1 F2 134.4(6) 5_555 1_555 ?
Ag1 F1 F2 132.1(6) 5_555 2_655 ?
Ag1 F1 F2 134.4(6) 5_555 3_565 ?
Ag1 F1 F2 132.1(6) 5_555 4_465 ?
Ag1 F1 F2 45.6(6) 5_555 5_555 ?
Ag1 F1 F2 47.9(6) 5_555 6_455 ?
Ag1 F1 F2 45.6(6) 5_555 7_565 ?
Ag1 F1 F2 47.9(6) 5_555 8_665 ?
F2 F1 F2 62.0(8) 1_555 2_655 ?
F2 F1 F2 91.1(11) 1_555 3_565 ?
F2 F1 F2 62.0(8) 1_555 4_465 ?
F2 F1 F2 119.3(8) 1_555 5_555 ?
F2 F1 F2 177.7(11) 1_555 6_455 ?
F2 F1 F2 119.3(8) 1_555 7_565 ?
F2 F1 F2 86.6(5) 1_555 8_665 ?
F2 F1 F2 62.0(8) 2_655 3_565 ?
F2 F1 F2 95.7(11) 2_655 4_465 ?
F2 F1 F2 177.7(11) 2_655 5_555 ?
F2 F1 F2 116.8(8) 2_655 6_455 ?
F2 F1 F2 86.6(5) 2_655 7_565 ?
F2 F1 F2 116.8(8) 2_655 8_665 ?
F2 F1 F2 62.0(8) 3_565 4_465 ?
F2 F1 F2 119.3(8) 3_565 5_555 ?
F2 F1 F2 86.6(5) 3_565 6_455 ?
F2 F1 F2 119.3(8) 3_565 7_565 ?
F2 F1 F2 177.7(11) 3_565 8_665 ?
F2 F1 F2 86.6(5) 4_465 5_555 ?
F2 F1 F2 116.8(8) 4_465 6_455 ?
F2 F1 F2 177.7(11) 4_465 7_565 ?
F2 F1 F2 116.8(8) 4_465 8_665 ?
F2 F1 F2 62.0(8) 5_555 6_455 ?
F2 F1 F2 91.1(11) 5_555 7_565 ?
F2 F1 F2 62.0(8) 5_555 8_665 ?
F2 F1 F2 62.0(8) 6_455 7_565 ?
F2 F1 F2 95.7(11) 6_455 8_665 ?
F2 F1 F2 62.0(8) 7_565 8_665 ?
Rb1 F2 Rb1 86.5(5) 1_565 5_564 ?
Rb1 F2 Rb1 176.7(5) 1_565 17_554 ?
Rb1 F2 Rb1 93.4(5) 1_565 21_555 ?
Rb1 F2 Ag1 91.7(8) 1_565 1_555 ?
Rb1 F2 Ag1 88.3(7) 1_565 2_665 ?
Rb1 F2 F1 62.7(5) 1_565 1_555 ?
Rb1 F2 F1 61.2(5) 1_565 2_665 ?
Rb1 F2 F1 120.0(5) 1_565 5_554 ?
Rb1 F2 F1 116.0(5) 1_565 6_564 ?
Rb1 F2 F2 123.7(11) 1_565 2_655 ?
Rb1 F2 F2 59.0(8) 1_565 2_665 ?
Rb1 F2 F2 59.0(8) 1_565 4_465 ?
Rb1 F2 F2 118.2(10) 1_565 4_565 ?
Rb1 F2 Rb1 93.4(5) 5_564 17_554 ?
Rb1 F2 Rb1 176.7(5) 5_564 21_555 ?
Rb1 F2 Ag1 91.7(8) 5_564 1_555 ?
Rb1 F2 Ag1 88.3(7) 5_564 2_665 ?
Rb1 F2 F1 120.0(5) 5_564 1_555 ?
Rb1 F2 F1 116.0(5) 5_564 2_665 ?
Rb1 F2 F1 62.7(5) 5_564 5_554 ?
Rb1 F2 F1 61.2(5) 5_564 6_564 ?
Rb1 F2 F2 123.7(11) 5_564 2_655 ?
Rb1 F2 F2 59.0(8) 5_564 2_665 ?
Rb1 F2 F2 59.0(8) 5_564 4_465 ?
Rb1 F2 F2 118.2(10) 5_564 4_565 ?
Rb1 F2 Rb1 86.5(5) 17_554 21_555 ?
Rb1 F2 Ag1 91.7(8) 17_554 1_555 ?
Rb1 F2 Ag1 88.3(7) 17_554 2_665 ?
Rb1 F2 F1 120.0(5) 17_554 1_555 ?
Rb1 F2 F1 116.0(5) 17_554 2_665 ?
Rb1 F2 F1 62.7(5) 17_554 5_554 ?
Rb1 F2 F1 61.2(5) 17_554 6_564 ?
Rb1 F2 F2 59.0(8) 17_554 2_655 ?
Rb1 F2 F2 118.2(10) 17_554 2_665 ?
Rb1 F2 F2 123.7(11) 17_554 4_465 ?
Rb1 F2 F2 59.0(8) 17_554 4_565 ?
Rb1 F2 Ag1 91.7(8) 21_555 1_555 ?
Rb1 F2 Ag1 88.3(7) 21_555 2_665 ?
Rb1 F2 F1 62.7(5) 21_555 1_555 ?
Rb1 F2 F1 61.2(5) 21_555 2_665 ?
Rb1 F2 F1 120.0(5) 21_555 5_554 ?
Rb1 F2 F1 116.0(5) 21_555 6_564 ?
Rb1 F2 F2 59.0(8) 21_555 2_655 ?
Rb1 F2 F2 118.2(10) 21_555 2_665 ?
Rb1 F2 F2 123.7(11) 21_555 4_465 ?
Rb1 F2 F2 59.0(8) 21_555 4_565 ?
Ag1 F2 Ag1 180.0(9) 1_555 2_665 ?
Ag1 F2 F1 137.9(8) 1_555 2_665 ?
Ag1 F2 F1 137.9(8) 1_555 6_564 ?
Ag1 F2 F2 47.3(11) 1_555 2_655 ?
Ag1 F2 F2 137.3(14) 1_555 2_665 ?
Ag1 F2 F2 47.3(11) 1_555 4_465 ?
Ag1 F2 F2 137.3(14) 1_555 4_565 ?
Ag1 F2 F1 135.6(7) 2_665 1_555 ?
Ag1 F2 F1 135.6(7) 2_665 5_554 ?
Ag1 F2 F2 132.7(13) 2_665 2_655 ?
Ag1 F2 F2 132.7(13) 2_665 4_465 ?
F1 F2 F1 93.4(5) 1_555 2_665 ?
F1 F2 F1 88.9(5) 1_555 5_554 ?
F1 F2 F1 177.7(5) 1_555 6_564 ?
F1 F2 F2 61.0(8) 1_555 2_655 ?
F1 F2 F2 121.6(11) 1_555 2_665 ?
F1 F2 F2 61.0(8) 1_555 4_465 ?
F1 F2 F2 121.6(11) 1_555 4_565 ?
F1 F2 F1 177.7(5) 2_665 5_554 ?
F1 F2 F1 84.3(5) 2_665 6_564 ?
F1 F2 F2 120.2(10) 2_665 2_655 ?
F1 F2 F2 57.0(8) 2_665 2_665 ?
F1 F2 F2 120.2(10) 2_665 4_465 ?
F1 F2 F2 57.0(8) 2_665 4_565 ?
F1 F2 F1 93.4(5) 5_554 6_564 ?
F1 F2 F2 61.0(8) 5_554 2_655 ?
F1 F2 F2 121.6(11) 5_554 2_665 ?
F1 F2 F2 61.0(8) 5_554 4_465 ?
F1 F2 F2 121.6(11) 5_554 4_565 ?
F1 F2 F2 120.2(10) 6_564 2_655 ?
F1 F2 F2 57.0(8) 6_564 2_665 ?
F1 F2 F2 120.2(10) 6_564 4_465 ?
F1 F2 F2 57.0(8) 6_564 4_565 ?
F2 F2 F2 175.4(16) 2_655 2_665 ?
F2 F2 F2 94.6(13) 2_655 4_465 ?
F2 F2 F2 90.0(13) 2_655 4_565 ?
F2 F2 F2 90.0(13) 2_665 4_465 ?
F2 F2 F2 85.4(13) 2_665 4_565 ?
F2 F2 F2 175.4(16) 4_465 4_565 ?

#=============================================================================


#=============================================================================
# Additional structures (last six sections and associated data_? identifiers) 
# may be added at this point.                                                 
#=============================================================================

# The following lines are used to test the character set of files sent by     
# network email or other means. They are not part of the CIF data set.        
# abcdefghijklmnopqrstuvwxyzABCDEFGHIJKLMNOPQRSTUVWXYZ0123456789              
# !@#$%^&*()_+{}:"~<>?|\-=[];'`,./ 
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_Rb3Ag2F7
_database_code_depnum_ccdc_archive 'CCDC 2122450'
loop_
_audit_author_name
_audit_author_address
'Kacper Koteras'
;Centre of New Technologies, University of Warsaw
Poland
;
_audit_update_record             
;
2021-12-21 deposited with the CCDC.	2021-12-23 downloaded from the CCDC.
;
# start Validation Reply Form
_vrf_PLAT112_Rb3Ag2F7            
;
PROBLEM: ADDSYM Detects New (Pseudo) Symm. Elem         4        100 %Fit
RESPONSE: Look at "PLAT113" response.
;
_vrf_PLAT112_Rb3Ag2F7_2          
;
PROBLEM: ADDSYM Detects New (Pseudo) Symm. Elem         m        100 %Fit
RESPONSE: Look at "PLAT113" response.
;
_vrf_PLAT112_Rb3Ag2F7_3          
;
PROBLEM: ADDSYM Detects New (Pseudo) Symm. Elem         m        100 %Fit
RESPONSE: Look at "PLAT113" response.
;
_vrf_PLAT113_Rb3Ag2F7            
;
PROBLEM: ADDSYM Suggests Possible Pseudo/New  Space Group     I4/mmm Check
RESPONSE: The primitive cell suggested by this alert is certainly wrong as it has equal equatorial Ag-F bonds within AgF2 sheets; this does not happen in any compound of Ag(II) since - due to cooperative Jahn-Teller effect - the Ag-F bond pattern is antiferrodistortive, i.e. long-short-long-short etc. The only exception from that would be a system with strong substitutional disorder reflected by two distinct positions of F atoms inside the plane, both occupied with 50% probability. this model is hard to be differentiated from our model solely in a Rietveld fit. as we see no support for such a disordered model from other methods we decided to use ordered cell.
;
_vrf_REFI015_Rb3Ag2F7            
;
PROBLEM: _refine_ls_shift/su_max is missing
RESPONSE: FullProf software doesn?t provide that particular parameter, as it reports them equal to zero after reaching convergence.
;
_vrf_PLAT732_Rb3Ag2F7            
;
PROBLEM: Angle   Calc    130.0(8), Rep      130(2) ......       2.50 s.u.-R
RESPONSE: This is caused by Fullprof numerical methods.
;
_vrf_PLAT741_Rb3Ag2F7            
;
PROBLEM: Bond    Calc   3.1791(7), Rep     3.17905 ......    Missing s.u.
RESPONSE: This are the distances between atoms in special positions, so FullProf doesn?t add standard uncertainties to them.
;
_vrf_PLAT741_Rb3Ag2F7_2          
;
PROBLEM: Bond    Calc   3.1791(7), Rep     3.17905 ......    Missing s.u.
RESPONSE: This are the distances between atoms in special positions, so FullProf doesn?t add standard uncertainties to them.
;
_vrf_PLAT741_Rb3Ag2F7_3          
;
PROBLEM: Bond    Calc   3.1788(7), Rep     3.17880 ......    Missing s.u.
RESPONSE: This are the distances between atoms in special positions, so FullProf doesn?t add standard uncertainties to them.
;
_vrf_PLAT741_Rb3Ag2F7_4          
;
PROBLEM: Bond    Calc   3.1788(7), Rep     3.17880 ......    Missing s.u.
RESPONSE: This are the distances between atoms in special positions, so FullProf doesn?t add standard uncertainties to them.
;
_vrf_PLAT741_Rb3Ag2F7_5          
;
PROBLEM: Bond    Calc   3.1791(7), Rep     3.17905 ......    Missing s.u.
RESPONSE: This are the distances between atoms in special positions, so FullProf doesn?t add standard uncertainties to them.
;
_vrf_PLAT741_Rb3Ag2F7_6          
;
PROBLEM: Bond    Calc   3.1791(7), Rep     3.17905 ......    Missing s.u.
RESPONSE: This are the distances between atoms in special positions, so FullProf doesn?t add standard uncertainties to them.
;
_vrf_PLAT741_Rb3Ag2F7_7          
;
PROBLEM: Bond    Calc   3.1788(7), Rep     3.17880 ......    Missing s.u.
RESPONSE: This are the distances between atoms in special positions, so FullProf doesn?t add standard uncertainties to them.
;
_vrf_PLAT741_Rb3Ag2F7_8          
;
PROBLEM: Bond    Calc   3.1788(7), Rep     3.17880 ......    Missing s.u.
RESPONSE: This are the distances between atoms in special positions, so FullProf doesn?t add standard uncertainties to them.
;
# Added during the CSD deposition process: Tuesday 21 December 2021 12:42 PM
# end Validation Reply Form


#=============================================================================

# 5. CHEMICAL DATA

_chemical_name_systematic        'Trirubidium heptafuoro diargenate(II)'
_chemical_formula_structural     'Ag2 F7 Rb3'
_chemical_formula_iupac          'Ag2 F7 Rb3'
_chemical_formula_sum            'Ag2 F7 Rb3'
_chemical_formula_weight         605.1282
_exptl_crystal_density_diffrn    4.5701


#=============================================================================

# 6. POWDER SPECIMEN AND CRYSTAL DATA

_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_H-M   'C m c a'
_symmetry_space_group_name_Hall  '-C 2bc 2'

loop_
_symmetry_equiv_pos_as_xyz #<--must include 'x,y,z'
x,y,z
x+1/2,-y+1/2,-z
-x+1/2,y,-z+1/2
-x,-y+1/2,z+1/2
-x,-y,-z
-x+1/2,y+1/2,z
x+1/2,-y,z+1/2
x,y+1/2,-z+1/2
x+1/2,y+1/2,z
x,-y,-z
-x,y+1/2,-z+1/2
-x+1/2,-y,z+1/2
-x+1/2,-y+1/2,-z
-x,y,z
x,-y+1/2,z+1/2
x+1/2,y,-z+1/2


_cell_length_a                   21.7581(5)
_cell_length_b                   6.3581(13)
_cell_length_c                   6.3576(13)
_cell_angle_alpha                90.0000
_cell_angle_beta                 90.0000
_cell_angle_gamma                90.0000
_cell_volume                     879.5(3)
_cell_formula_units_Z            4
_cell_measurement_temperature    293
_cell_special_details            ?


# The next five fields are character fields that describe the specimen.

_pd_spec_mounting                capillary # This field should be
# used to give details of the 
# container.
_pd_spec_mount_mode              transmission # options are 'reflection'
# or 'transmission'
_pd_spec_shape                   cylinder # options are 'cylinder' 
# 'flat_sheet' or 'irregular'
_pd_char_colour                  brown # use ICDD colour descriptions



#=============================================================================

# 7. EXPERIMENTAL DATA


# The following item is used to identify the equipment used to record 
# the powder pattern when the diffractogram was measured at a laboratory 
# other than the authors' home institution, e.g. when neutron or synchrotron
# radiation is used.

_diffrn_ambient_temperature      293
_diffrn_radiation_type           'Cu K\a'

_diffrn_radiation_monochromator  none
_diffrn_measurement_device_type  'Bruker D8 DISCOVER'
_diffrn_measurement_method       capillary
_pd_meas_scan_method             step # options are 'step', 'cont',
# 'tof', 'fixed' or
# 'disp' (= dispersive)
_pd_meas_special_details         ?

#  The following four items give details of the measured (not processed)
#  powder pattern.  Angles are in degrees.

_pd_meas_number_of_points        5866
_pd_meas_2theta_range_min        6.01430
_pd_meas_2theta_range_max        89.86021
_pd_meas_2theta_range_inc        0.014299

#=============================================================================

# 8. REFINEMENT DATA

_refine_special_details          ?

# Use the next field to give any special details about the fitting of the
# powder pattern.

_pd_proc_ls_special_details      ?

# The next three items are given as text.

_pd_proc_ls_profile_function     ?
_pd_proc_ls_background_function  ?
_pd_proc_ls_pref_orient_corr     ?

#  The following profile R-factors are NOT CORRECTED for background
#  The sum is extended to all non-excluded points.
#  These are the current CIF standard

_pd_proc_ls_prof_R_factor        0.8494
_pd_proc_ls_prof_wR_factor       1.8355
_pd_proc_ls_prof_wR_expected     0.5932


#  Items related to LS refinement

_refine_ls_goodness_of_fit_all   3.094
_refine_ls_R_I_factor            5.6897
_refine_ls_number_reflns         387
_refine_ls_number_parameters     26
_refine_ls_number_restraints     0

# The following four items apply to angular dispersive measurements.
# 2theta minimum, maximum and increment (in degrees) are for the 
# intensities used in the refinement.

_pd_proc_2theta_range_min        6.0151
_pd_proc_2theta_range_max        89.8610
_pd_proc_2theta_range_inc        0.014299
_pd_proc_wavelength              1.540560


loop_
_pd_block_diffractogram_id
?
# The id used for the block containing
# the powder pattern profile (section 11)

# Give appropriate details in the next two text fields.

_pd_proc_info_excluded_regions   none
_pd_proc_info_data_reduction     none

# The following items are used to identify the programs used.

_computing_data_collection       ?
_computing_structure_solution    ?
_computing_structure_refinement  FULLPROF
_computing_molecular_graphics    ?
_computing_publication_material  ?

#=============================================================================

# 9. ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS

loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_occupancy
_atom_site_adp_type
_atom_site_type_symbol

Rb1 0.68400(18) 0.00000 0.00000 0.010(2) 1.00000 Uiso Rb
Rb2 0.50000 0.00000 0.00000 0.011(3) 1.00000 Uiso Rb
Ag1 -0.0965(2) 0.00000 0.00000 0.0143(14) 1.00000 Uiso Ag
F1 0.8045(15) 0.00000 0.00000 0.067(10) 1.00000 Uiso F
F2 0.00000 0.00000 0.00000 0.018(11) 1.00000 Uiso F
F3 0.5899(7) 0.275(12) 0.268(10) 0.001(6) 1.00000 Uiso F

# Note: if the displacement parameters were refined anisotropically
# the U matrices should be given as for single-crystal studies.

#=============================================================================

# 10. DISTANCES AND ANGLES / MOLECULAR GEOMETRY 
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Rb1 F1 2.62(3) 1_555 ?
Rb1 F1 3.189(3) 3_654 ?
Rb1 F1 3.189(3) 3_655 ?
Rb1 F1 3.189(3) 6_645 ?
Rb1 F1 3.189(3) 6_655 ?
Rb1 F3 3.19(5) 1_555 ?
Rb1 F3 2.90(5) 8_545 ?
Rb1 F3 3.19(5) 10_555 ?
Rb1 F3 2.90(5) 15_554 ?
Rb2 F2 3.17905 2_545 ?
Rb2 F2 3.17905 2_555 ?
Rb2 F2 3.17880 3_554 ?
Rb2 F2 3.17880 3_555 ?
Rb2 F3 3.13(6) 1_555 ?
Rb2 F3 2.84(5) 4_654 ?
Rb2 F3 3.13(6) 5_655 ?
Rb2 F3 2.84(5) 8_545 ?
Rb2 F3 3.13(6) 10_555 ?
Rb2 F3 2.84(5) 11_645 ?
Rb2 F3 3.13(6) 14_655 ?
Rb2 F3 2.84(5) 15_554 ?
Ag1 F1 2.15(3) 1_455 ?
Ag1 F2 2.100(4) 1_555 ?
Ag1 F3 2.29(7) 3_555 ?
Ag1 F3 2.23(7) 6_545 ?
Ag1 F3 2.29(7) 12_554 ?
Ag1 F3 2.23(7) 13_555 ?
F1 Rb1 2.62(3) 1_555 ?
F1 Rb1 3.189(3) 3_654 ?
F1 Rb1 3.189(3) 3_655 ?
F1 Rb1 3.189(3) 6_645 ?
F1 Rb1 3.189(3) 6_655 ?
F1 Ag1 2.15(3) 1_655 ?
F1 F3 3.24(6) 3_655 ?
F1 F3 3.20(5) 6_645 ?
F1 F3 3.24(6) 12_654 ?
F1 F3 3.20(5) 13_655 ?
F2 Rb2 3.17905 2_445 ?
F2 Rb2 3.17905 2_455 ?
F2 Rb2 3.17880 3_554 ?
F2 Rb2 3.17880 3_555 ?
F2 Ag1 2.100(4) 1_555 ?
F2 Ag1 2.100(4) 5_555 ?
F2 F3 2.96(5) 2_455 ?
F2 F3 3.01(6) 3_555 ?
F2 F3 2.96(5) 6_545 ?
F2 F3 3.01(6) 7_454 ?
F2 F3 2.96(5) 9_445 ?
F2 F3 3.01(6) 12_554 ?
F2 F3 2.96(5) 13_555 ?
F2 F3 3.01(6) 16_455 ?
F3 Rb1 3.19(5) 1_555 ?
F3 Rb1 2.90(5) 8_555 ?
F3 Rb2 3.13(6) 1_555 ?
F3 Rb2 2.84(5) 4_655 ?
F3 Ag1 2.29(7) 3_555 ?
F3 Ag1 2.23(7) 6_555 ?
F3 F1 3.24(6) 3_655 ?
F3 F1 3.20(5) 6_655 ?
F3 F2 2.96(5) 2_555 ?
F3 F2 3.01(6) 3_555 ?
F3 F3 3.19(11) 8_545 ?
F3 F3 3.19(11) 8_555 ?
F3 F3 3.19(9) 15_554 ?
F3 F3 3.19(9) 15_555 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
F1 Rb1 F1 85.5(10) 1_555 3_654 ?
F1 Rb1 F1 85.5(10) 1_555 3_655 ?
F1 Rb1 F1 85.5(10) 1_555 6_645 ?
F1 Rb1 F1 85.5(10) 1_555 6_655 ?
F1 Rb1 F3 130(2) 1_555 1_555 ?
F1 Rb1 F3 135(2) 1_555 8_545 ?
F1 Rb1 F3 130(2) 1_555 10_555 ?
F1 Rb1 F3 135(2) 1_555 15_554 ?
F1 Rb1 F1 171.00(7) 3_654 3_655 ?
F1 Rb1 F1 89.65(7) 3_654 6_645 ?
F1 Rb1 F1 89.65(7) 3_654 6_655 ?
F1 Rb1 F3 126(2) 3_654 1_555 ?
F1 Rb1 F3 124(2) 3_654 8_545 ?
F1 Rb1 F3 61.1(14) 3_654 10_555 ?
F1 Rb1 F3 63.2(15) 3_654 15_554 ?
F1 Rb1 F1 89.65(7) 3_655 6_645 ?
F1 Rb1 F1 89.65(7) 3_655 6_655 ?
F1 Rb1 F3 61.1(14) 3_655 1_555 ?
F1 Rb1 F3 63.2(15) 3_655 8_545 ?
F1 Rb1 F3 126(2) 3_655 10_555 ?
F1 Rb1 F3 124(2) 3_655 15_554 ?
F1 Rb1 F1 171.00(7) 6_645 6_655 ?
F1 Rb1 F3 127(2) 6_645 1_555 ?
F1 Rb1 F3 64.1(15) 6_645 8_545 ?
F1 Rb1 F3 60.2(14) 6_645 10_555 ?
F1 Rb1 F3 123(3) 6_645 15_554 ?
F1 Rb1 F3 60.2(14) 6_655 1_555 ?
F1 Rb1 F3 123(3) 6_655 8_545 ?
F1 Rb1 F3 127(2) 6_655 10_555 ?
F1 Rb1 F3 64.1(15) 6_655 15_554 ?
F3 Rb1 F3 63(3) 1_555 8_545 ?
F3 Rb1 F3 100(3) 1_555 10_555 ?
F3 Rb1 F3 63(2) 1_555 15_554 ?
F3 Rb1 F3 63(2) 8_545 10_555 ?
F3 Rb1 F3 90(3) 8_545 15_554 ?
F3 Rb1 F3 63(3) 10_555 15_554 ?
F2 Rb2 F2 180.000 2_545 2_555 ?
F2 Rb2 F2 90.0000 2_545 3_554 ?
F2 Rb2 F2 90.0000 2_545 3_555 ?
F2 Rb2 F3 124(2) 2_545 1_555 ?
F2 Rb2 F3 120(3) 2_545 4_654 ?
F2 Rb2 F3 56.0(14) 2_545 5_655 ?
F2 Rb2 F3 59.7(15) 2_545 8_545 ?
F2 Rb2 F3 56.0(14) 2_545 10_555 ?
F2 Rb2 F3 59.7(15) 2_545 11_645 ?
F2 Rb2 F3 124(2) 2_545 14_655 ?
F2 Rb2 F3 120(3) 2_545 15_554 ?
F2 Rb2 F2 90.0000 2_555 3_554 ?
F2 Rb2 F2 90.0000 2_555 3_555 ?
F2 Rb2 F3 56.0(14) 2_555 1_555 ?
F2 Rb2 F3 59.7(15) 2_555 4_654 ?
F2 Rb2 F3 124(2) 2_555 5_655 ?
F2 Rb2 F3 120(3) 2_555 8_545 ?
F2 Rb2 F3 124(2) 2_555 10_555 ?
F2 Rb2 F3 120(3) 2_555 11_645 ?
F2 Rb2 F3 56.0(14) 2_555 14_655 ?
F2 Rb2 F3 59.7(15) 2_555 15_554 ?
F2 Rb2 F2 179.972 3_554 3_555 ?
F2 Rb2 F3 123(2) 3_554 1_555 ?
F2 Rb2 F3 58.7(14) 3_554 4_654 ?
F2 Rb2 F3 57.0(14) 3_554 5_655 ?
F2 Rb2 F3 121(2) 3_554 8_545 ?
F2 Rb2 F3 57.0(14) 3_554 10_555 ?
F2 Rb2 F3 121(2) 3_554 11_645 ?
F2 Rb2 F3 123(2) 3_554 14_655 ?
F2 Rb2 F3 58.7(14) 3_554 15_554 ?
F2 Rb2 F3 57.0(14) 3_555 1_555 ?
F2 Rb2 F3 121(2) 3_555 4_654 ?
F2 Rb2 F3 123(2) 3_555 5_655 ?
F2 Rb2 F3 58.7(14) 3_555 8_545 ?
F2 Rb2 F3 123(2) 3_555 10_555 ?
F2 Rb2 F3 58.7(14) 3_555 11_645 ?
F2 Rb2 F3 57.0(14) 3_555 14_655 ?
F2 Rb2 F3 121(2) 3_555 15_554 ?
F3 Rb2 F3 116(2) 1_555 4_654 ?
F3 Rb2 F3 180(3) 1_555 5_655 ?
F3 Rb2 F3 64(3) 1_555 8_545 ?
F3 Rb2 F3 103(3) 1_555 10_555 ?
F3 Rb2 F3 115(3) 1_555 11_645 ?
F3 Rb2 F3 77.4(15) 1_555 14_655 ?
F3 Rb2 F3 65(2) 1_555 15_554 ?
F3 Rb2 F3 64(3) 4_654 5_655 ?
F3 Rb2 F3 180(3) 4_654 8_545 ?
F3 Rb2 F3 115(3) 4_654 10_555 ?
F3 Rb2 F3 93(3) 4_654 11_645 ?
F3 Rb2 F3 65(2) 4_654 14_655 ?
F3 Rb2 F3 87.2(16) 4_654 15_554 ?
F3 Rb2 F3 116(2) 5_655 8_545 ?
F3 Rb2 F3 77.4(15) 5_655 10_555 ?
F3 Rb2 F3 65(2) 5_655 11_645 ?
F3 Rb2 F3 103(3) 5_655 14_655 ?
F3 Rb2 F3 115(3) 5_655 15_554 ?
F3 Rb2 F3 65(2) 8_545 10_555 ?
F3 Rb2 F3 87.2(16) 8_545 11_645 ?
F3 Rb2 F3 115(3) 8_545 14_655 ?
F3 Rb2 F3 93(3) 8_545 15_554 ?
F3 Rb2 F3 116(2) 10_555 11_645 ?
F3 Rb2 F3 180(3) 10_555 14_655 ?
F3 Rb2 F3 64(3) 10_555 15_554 ?
F3 Rb2 F3 64(3) 11_645 14_655 ?
F3 Rb2 F3 180(3) 11_645 15_554 ?
F3 Rb2 F3 116(2) 14_655 15_554 ?
F1 Ag1 F2 180.0(20) 1_455 1_555 ?
F1 Ag1 F3 94(3) 1_455 3_555 ?
F1 Ag1 F3 94(3) 1_455 6_545 ?
F1 Ag1 F3 94(3) 1_455 12_554 ?
F1 Ag1 F3 94(3) 1_455 13_555 ?
F2 Ag1 F3 86(3) 1_555 3_555 ?
F2 Ag1 F3 86(3) 1_555 6_545 ?
F2 Ag1 F3 86(3) 1_555 12_554 ?
F2 Ag1 F3 86(3) 1_555 13_555 ?
F3 Ag1 F3 90(5) 3_555 6_545 ?
F3 Ag1 F3 173(6) 3_555 12_554 ?
F3 Ag1 F3 90(4) 3_555 13_555 ?
F3 Ag1 F3 90(4) 6_545 12_554 ?
F3 Ag1 F3 173(6) 6_545 13_555 ?
F3 Ag1 F3 90(5) 12_554 13_555 ?
Rb1 F1 Rb1 94.5(7) 1_555 3_654 ?
Rb1 F1 Rb1 94.5(7) 1_555 3_655 ?
Rb1 F1 Rb1 94.5(7) 1_555 6_645 ?
Rb1 F1 Rb1 94.5(7) 1_555 6_655 ?
Rb1 F1 Ag1 180.0(12) 1_555 1_655 ?
Rb1 F1 F3 135.1(17) 1_555 3_655 ?
Rb1 F1 F3 135.9(17) 1_555 6_645 ?
Rb1 F1 F3 135.1(17) 1_555 12_654 ?
Rb1 F1 F3 135.9(17) 1_555 13_655 ?
Rb1 F1 Rb1 171.00(7) 3_654 3_655 ?
Rb1 F1 Rb1 89.65(7) 3_654 6_645 ?
Rb1 F1 Rb1 89.65(7) 3_654 6_655 ?
Rb1 F1 Ag1 85.5(9) 3_654 1_655 ?
Rb1 F1 F3 113(2) 3_654 3_655 ?
Rb1 F1 F3 118(2) 3_654 6_645 ?
Rb1 F1 F3 59.4(14) 3_654 12_654 ?
Rb1 F1 F3 54.0(13) 3_654 13_655 ?
Rb1 F1 Rb1 89.65(7) 3_655 6_645 ?
Rb1 F1 Rb1 89.65(7) 3_655 6_655 ?
Rb1 F1 Ag1 85.5(9) 3_655 1_655 ?
Rb1 F1 F3 59.4(14) 3_655 3_655 ?
Rb1 F1 F3 54.0(13) 3_655 6_645 ?
Rb1 F1 F3 113(2) 3_655 12_654 ?
Rb1 F1 F3 118(2) 3_655 13_655 ?
Rb1 F1 Rb1 171.00(7) 6_645 6_655 ?
Rb1 F1 Ag1 85.5(9) 6_645 1_655 ?
Rb1 F1 F3 119(2) 6_645 3_655 ?
Rb1 F1 F3 59.8(14) 6_645 6_645 ?
Rb1 F1 F3 53.6(13) 6_645 12_654 ?
Rb1 F1 F3 113(2) 6_645 13_655 ?
Rb1 F1 Ag1 85.5(9) 6_655 1_655 ?
Rb1 F1 F3 53.6(13) 6_655 3_655 ?
Rb1 F1 F3 113(2) 6_655 6_645 ?
Rb1 F1 F3 119(2) 6_655 12_654 ?
Rb1 F1 F3 59.8(14) 6_655 13_655 ?
F3 F1 F3 59(2) 3_655 6_645 ?
F3 F1 F3 90(3) 3_655 12_654 ?
F3 F1 F3 59(2) 3_655 13_655 ?
F3 F1 F3 59(2) 6_645 12_654 ?
F3 F1 F3 88(3) 6_645 13_655 ?
F3 F1 F3 59(2) 12_654 13_655 ?
Rb2 F2 Rb2 180.000 2_445 2_455 ?
Rb2 F2 Rb2 90.0000 2_445 3_554 ?
Rb2 F2 Rb2 90.0000 2_445 3_555 ?
Rb2 F2 Ag1 90.00(14) 2_445 1_555 ?
Rb2 F2 Ag1 90.00(14) 2_445 5_555 ?
Rb2 F2 F3 119(2) 2_445 2_455 ?
Rb2 F2 F3 126(3) 2_445 3_555 ?
Rb2 F2 F3 61.1(15) 2_445 6_545 ?
Rb2 F2 F3 54.5(14) 2_445 7_454 ?
Rb2 F2 F3 61.1(15) 2_445 9_445 ?
Rb2 F2 F3 54.5(14) 2_445 12_554 ?
Rb2 F2 F3 119(2) 2_445 13_555 ?
Rb2 F2 F3 126(3) 2_445 16_455 ?
Rb2 F2 Rb2 90.0000 2_455 3_554 ?
Rb2 F2 Rb2 90.0000 2_455 3_555 ?
Rb2 F2 Ag1 90.00(14) 2_455 1_555 ?
Rb2 F2 Ag1 90.00(14) 2_455 5_555 ?
Rb2 F2 F3 61.1(15) 2_455 2_455 ?
Rb2 F2 F3 54.5(14) 2_455 3_555 ?
Rb2 F2 F3 119(2) 2_455 6_545 ?
Rb2 F2 F3 126(3) 2_455 7_454 ?
Rb2 F2 F3 119(2) 2_455 9_445 ?
Rb2 F2 F3 126(3) 2_455 12_554 ?
Rb2 F2 F3 61.1(15) 2_455 13_555 ?
Rb2 F2 F3 54.5(14) 2_455 16_455 ?
Rb2 F2 Rb2 179.972 3_554 3_555 ?
Rb2 F2 Ag1 90.00(14) 3_554 1_555 ?
Rb2 F2 Ag1 90.00(14) 3_554 5_555 ?
Rb2 F2 F3 54.9(14) 3_554 2_455 ?
Rb2 F2 F3 119(2) 3_554 3_555 ?
Rb2 F2 F3 125(2) 3_554 6_545 ?
Rb2 F2 F3 60.7(15) 3_554 7_454 ?
Rb2 F2 F3 125(2) 3_554 9_445 ?
Rb2 F2 F3 60.7(15) 3_554 12_554 ?
Rb2 F2 F3 54.9(14) 3_554 13_555 ?
Rb2 F2 F3 119(2) 3_554 16_455 ?
Rb2 F2 Ag1 90.00(14) 3_555 1_555 ?
Rb2 F2 Ag1 90.00(14) 3_555 5_555 ?
Rb2 F2 F3 125(2) 3_555 2_455 ?
Rb2 F2 F3 60.7(15) 3_555 3_555 ?
Rb2 F2 F3 54.9(14) 3_555 6_545 ?
Rb2 F2 F3 119(2) 3_555 7_454 ?
Rb2 F2 F3 54.9(14) 3_555 9_445 ?
Rb2 F2 F3 119(2) 3_555 12_554 ?
Rb2 F2 F3 125(2) 3_555 13_555 ?
Rb2 F2 F3 60.7(15) 3_555 16_455 ?
Ag1 F2 Ag1 180.0(4) 1_555 5_555 ?
Ag1 F2 F3 131.3(18) 1_555 2_455 ?
Ag1 F2 F3 49.5(18) 1_555 3_555 ?
Ag1 F2 F3 48.7(18) 1_555 6_545 ?
Ag1 F2 F3 130.5(19) 1_555 7_454 ?
Ag1 F2 F3 131.3(18) 1_555 9_445 ?
Ag1 F2 F3 49.5(18) 1_555 12_554 ?
Ag1 F2 F3 48.7(18) 1_555 13_555 ?
Ag1 F2 F3 130.5(19) 1_555 16_455 ?
Ag1 F2 F3 48.7(18) 5_555 2_455 ?
Ag1 F2 F3 130.5(19) 5_555 3_555 ?
Ag1 F2 F3 131.3(18) 5_555 6_545 ?
Ag1 F2 F3 49.5(18) 5_555 7_454 ?
Ag1 F2 F3 48.7(18) 5_555 9_445 ?
Ag1 F2 F3 130.5(19) 5_555 12_554 ?
Ag1 F2 F3 131.3(18) 5_555 13_555 ?
Ag1 F2 F3 49.5(18) 5_555 16_455 ?
F3 F2 F3 115(2) 2_455 3_555 ?
F3 F2 F3 180(3) 2_455 6_545 ?
F3 F2 F3 65(3) 2_455 7_454 ?
F3 F2 F3 97(3) 2_455 9_445 ?
F3 F2 F3 115(3) 2_455 12_554 ?
F3 F2 F3 82.6(15) 2_455 13_555 ?
F3 F2 F3 65(2) 2_455 16_455 ?
F3 F2 F3 65(3) 3_555 6_545 ?
F3 F2 F3 180(3) 3_555 7_454 ?
F3 F2 F3 115(3) 3_555 9_445 ?
F3 F2 F3 99(3) 3_555 12_554 ?
F3 F2 F3 65(2) 3_555 13_555 ?
F3 F2 F3 81.1(16) 3_555 16_455 ?
F3 F2 F3 115(2) 6_545 7_454 ?
F3 F2 F3 82.6(15) 6_545 9_445 ?
F3 F2 F3 65(2) 6_545 12_554 ?
F3 F2 F3 97(3) 6_545 13_555 ?
F3 F2 F3 115(3) 6_545 16_455 ?
F3 F2 F3 65(2) 7_454 9_445 ?
F3 F2 F3 81.1(16) 7_454 12_554 ?
F3 F2 F3 115(3) 7_454 13_555 ?
F3 F2 F3 99(3) 7_454 16_455 ?
F3 F2 F3 115(2) 9_445 12_554 ?
F3 F2 F3 180(3) 9_445 13_555 ?
F3 F2 F3 65(3) 9_445 16_455 ?
F3 F2 F3 65(3) 12_554 13_555 ?
F3 F2 F3 180(3) 12_554 16_455 ?
F3 F2 F3 115(2) 13_555 16_455 ?
Rb1 F3 Rb1 95.1(14) 1_555 8_555 ?
Rb1 F3 Rb2 78.7(14) 1_555 1_555 ?
Rb1 F3 Rb2 176.2(14) 1_555 4_655 ?
Rb1 F3 Ag1 83(2) 1_555 3_555 ?
Rb1 F3 Ag1 84(2) 1_555 6_555 ?
Rb1 F3 F1 59.5(14) 1_555 3_655 ?
Rb1 F3 F1 59.9(14) 1_555 6_655 ?
Rb1 F3 F2 112.4(14) 1_555 2_555 ?
Rb1 F3 F2 111.2(14) 1_555 3_555 ?
Rb1 F3 F3 54(2) 1_555 8_545 ?
Rb1 F3 F3 121(3) 1_555 8_555 ?
Rb1 F3 F3 54(2) 1_555 15_554 ?
Rb1 F3 F3 119(3) 1_555 15_555 ?
Rb1 F3 Rb2 173.7(14) 8_555 1_555 ?
Rb1 F3 Rb2 88.5(15) 8_555 4_655 ?
Rb1 F3 Ag1 90(2) 8_555 3_555 ?
Rb1 F3 Ag1 92(2) 8_555 6_555 ?
Rb1 F3 F1 62.3(14) 8_555 3_655 ?
Rb1 F3 F1 62.8(14) 8_555 6_655 ?
Rb1 F3 F2 121.4(14) 8_555 2_555 ?
Rb1 F3 F2 119.7(15) 8_555 3_555 ?
Rb1 F3 F3 122(3) 8_555 8_545 ?
Rb1 F3 F3 63(2) 8_555 8_555 ?
Rb1 F3 F3 124(3) 8_555 15_554 ?
Rb1 F3 F3 63(2) 8_555 15_555 ?
Rb2 F3 Rb2 97.7(15) 1_555 4_655 ?
Rb2 F3 Ag1 88(2) 1_555 3_555 ?
Rb2 F3 Ag1 89(2) 1_555 6_555 ?
Rb2 F3 F1 112.9(16) 1_555 3_655 ?
Rb2 F3 F1 114.1(16) 1_555 6_655 ?
Rb2 F3 F2 62.9(14) 1_555 2_555 ?
Rb2 F3 F2 62.3(15) 1_555 3_555 ?
Rb2 F3 F3 53(2) 1_555 8_545 ?
Rb2 F3 F3 121(3) 1_555 8_555 ?
Rb2 F3 F3 53(2) 1_555 15_554 ?
Rb2 F3 F3 119(3) 1_555 15_555 ?
Rb2 F3 Ag1 95(2) 4_655 3_555 ?
Rb2 F3 Ag1 97(2) 4_655 6_555 ?
Rb2 F3 F1 121.6(17) 4_655 3_655 ?
Rb2 F3 F1 123.1(17) 4_655 6_655 ?
Rb2 F3 F2 66.4(15) 4_655 2_555 ?
Rb2 F3 F2 65.8(15) 4_655 3_555 ?
Rb2 F3 F3 123(3) 4_655 8_545 ?
Rb2 F3 F3 62(2) 4_655 8_555 ?
Rb2 F3 F3 125(3) 4_655 15_554 ?
Rb2 F3 F3 62(2) 4_655 15_555 ?
Ag1 F3 Ag1 168(3) 3_555 6_555 ?
Ag1 F3 F1 130(2) 3_555 6_655 ?
Ag1 F3 F2 141(2) 3_555 2_555 ?
Ag1 F3 F3 144(4) 3_555 8_555 ?
Ag1 F3 F3 124(3) 3_555 15_554 ?
Ag1 F3 F1 130(2) 6_555 3_655 ?
Ag1 F3 F2 45(2) 6_555 2_555 ?
Ag1 F3 F2 142(2) 6_555 3_555 ?
Ag1 F3 F3 126(4) 6_555 8_545 ?
Ag1 F3 F3 46(3) 6_555 8_555 ?
Ag1 F3 F3 46(3) 6_555 15_554 ?
Ag1 F3 F3 146(4) 6_555 15_555 ?
F1 F3 F1 88.5(14) 3_655 6_655 ?
F1 F3 F2 171.9(17) 3_655 2_555 ?
F1 F3 F2 85.7(17) 3_655 3_555 ?
F1 F3 F3 60(2) 3_655 8_545 ?
F1 F3 F3 125(3) 3_655 8_555 ?
F1 F3 F3 114(3) 3_655 15_554 ?
F1 F3 F3 60(2) 3_655 15_555 ?
F1 F3 F2 87.2(16) 6_655 2_555 ?
F1 F3 F2 171.0(17) 6_655 3_555 ?
F1 F3 F3 114(3) 6_655 8_545 ?
F1 F3 F3 61(2) 6_655 8_555 ?
F1 F3 F3 61(2) 6_655 15_554 ?
F1 F3 F3 125(3) 6_655 15_555 ?
F2 F3 F2 97.7(15) 2_555 3_555 ?
F2 F3 F3 116(3) 2_555 8_545 ?
F2 F3 F3 58(2) 2_555 8_555 ?
F2 F3 F3 58(2) 2_555 15_554 ?
F2 F3 F3 128(3) 2_555 15_555 ?
F2 F3 F3 57(2) 3_555 8_545 ?
F2 F3 F3 128(3) 3_555 8_555 ?
F2 F3 F3 115(3) 3_555 15_554 ?
F2 F3 F3 57(2) 3_555 15_555 ?
F3 F3 F3 172(5) 8_545 8_555 ?
F3 F3 F3 80(3) 8_545 15_554 ?
F3 F3 F3 88(4) 8_545 15_555 ?
F3 F3 F3 92(4) 8_555 15_554 ?
F3 F3 F3 100(4) 8_555 15_555 ?
F3 F3 F3 169(4) 15_554 15_555 ?

#=============================================================================




#=============================================================================
# Additional structures (last six sections and associated data_? identifiers) 
# may be added at this point.                                                 
#=============================================================================

# The following lines are used to test the character set of files sent by     
# network email or other means. They are not part of the CIF data set.        
# abcdefghijklmnopqrstuvwxyzABCDEFGHIJKLMNOPQRSTUVWXYZ0123456789              
# !@#$%^&*()_+{}:"~<>?|\-=[];'`,./ 
